{'fraction_non_alphanumeric': 0.08089260808926081, 'fraction_numerical': 0.027196652719665274, 'mean_word_length': 4.954356846473029, 'pattern_counts': {'":': 0, '<': 1, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
In situ study of the solid-state formation of U(1-x)Am(x)O(2±δ) solid solution.

In order to reduce the nuclear waste inventory and radiotoxicity, U(1-x)Am(x)O(2±δ) materials are promising fuels for heterogeneous transmutation. In this context, they are generally fabricated from UO(2+δ) and AmO(2-δ) dioxide powders. In the subsequent solid solution, americium is assumed to be trivalent whereas uranium exhibits a mixed-valence (+IV/+V) state. However, no formation mechanisms were ever evidenced and, more particularly, it was not possible to know whether the reduction of Am(IV) to Am(III) occurs before the solid-solution formation, or only once it is established. In this study, we used high-temperature X-ray diffraction on a UO(2±δ)/AmO(2-δ) (15 mol %) mixture to observe in situ the formation of the U(1-x)Am(x)O(2±δ) solid solution. We show that UO(2+δ) is, at relatively low temperature (<700 K), oxidized to U(4)O(9-δ), which is likely to be caused by oxygen release from the simultaneous AmO(2-δ) reduction to cubic Am(2)O(3±δ). Cubic Am(2)O(3+δ) then transforms to hexagonal Am(2)O(3) at 1300 K. Thus, the initial Am(IV) is fully reduced to Am(III) before the solid solution starts forming at 1740 K. The UO(2) fluorite phase vanishes after 4 h at 1970 K, indicating that the formation of the solid solution is completed, which proves that this solid solution is formed after the complete reduction of Am(IV) to Am(III).